bis 455 - portland slag cement specification
Post on 29-Nov-2014
Embed Size (px)
IS 455: 1888
SLAG CEMENT-SPECIFICATION( Fourth Revision )
Second Reprint SEPTEMBER 1998 UDC 666943
@ BIS 1990
INDIANBAHADUR NEW DELHI
STANDARDSSHAH 110002 e-4 ZAFAR MARG
Cenmnt and Concrete Sectional Committee, CED 2
FOREWORD This Indian Standard ( Fourth Revision ) was adopted by the Bureau of Indian Standards on 30 October 1989, after the draft finalized by the Cement .and Concrete Sectional Committee had been approved by the Civil Engineering Division Council. Portland slag cement is obtained by mixing, Portland cement clinker, gypsum and granulated slag in suitable proportions and grinding the mixture to get a thorough and intimate mix between the constituents. It may also be manufactured by separately grinding Portland cement clinker, gypsum and granulated slag and then mixing them intimately.. The resultant product is a cement which has physical properties similar to those of ordinary Portland cement. In addition, it has low heat of hydration and is relatively better resistant to soils and water containing excessive amounts of sulphater of alkali metals. alumina and iron, as well- as to acidic waters, and can, therefore, be used for marine works with advantage. The manufacture of Portland slag cement has been developed primarily to utilize blastfumace slag, a waste product from blastfurnaces. The development of manufacture of this type of cement will considerably increase the total output of cement production in the country and will, in addition, provide a profitable use for an otherwise waste product. The slags obtained from other types of furnaces, but having identical properties as those of granulated blastfumace slag conforming to this standard, may also be used for manufacture of Portland slag cement. This standard was first published in lb53 and subsequently revised in 1962,1967 and 1976. This fourth revision incorporates the modifications required as a result of experience gained with the use of this specification and to bring the standard in line with tlse present practices followed in the production and testing of cement. Since publication of the third revision of this standard, large number of amendments have been issued from time to time in order to modify various requirements based on the experience gained with the use of the standard and the requirements of the users and also keeping in view the raw materials and fuel available in the country for manufacture of cement. The important amendments include incorporating a value of 28 day compressive strength, increasing the requirement regarding loss on ignition from 40 to 50, increasing the insoluble residue content from 25 to 4 percent, making aumdave soundness test compulsory, incorpoiating a provision for retest in respect of autoclave soundness test after aeration of the cement, incorporating a clause on false set of cement and permitting packaging of cement in 25 kg bags. In view of these large number of amendments, the Sectiolral Committee decided to bring out the fourth revision of the standard incorporating all these amendments so as to make it more convenient for the users. The desirable requirements of granulated slag suitable for the manufacture of Portland slag cement have been deleted from this revision and reference has been made to IS 12089 : 1987 Specification for granulated slag for the manufacture of Portland slag cement. This standard contains clauses 5.1 and 11.4.1 which permit the purchaser to use his option and clauses 6.5,9.2.1 and 9.3 which call for agreement between the purchaser and the manufacturer. In the formulation of this standard considerable assistance has been rendered by National Corncil for Cement and Building Materials, New Delhi as many of these modifications are based on studies carried out by them. The composition of the committee responsible for the formulation of this standard is given in Annex C.
Mass of cement packed in bags and the tolerance requirements shall be in accordance with the relevant provisions of the Standards of Weights and Measures ( Packaged Commodities ) Rules, 1977 and,B-1.2 ( see Annex B for information ). Any modification in these rules in respect of tolerance on mass of cement would apply automatically to this standard. For the purpose of deciding whether a particular requirement of this standard is complied with, the final value, observed or calculated, expressing the result of a test or analysis, shall be rounded off in accordance with IS 2 : 1960 Rules for rounding off numerical values ( r&vised ). The number of significant places retained in the rounded off value should be the same as that of the specified value in this standard.
Is 395 : 1999
PORTLAND SLAG CEMENT - SPECIFICATION( Fourth Revision )1 SCOPE 1.1 This standard covers the manufacture and chemical and physical requirements for Portland slag cement. 2 REFERENCES 2.1 The Indian Standards listed in Annex A are necessary adjuncts to this standard. 3 TERMINOLOGY 3.1 For the purpose of this standard, the definitions given in 1S 4845 : 1968 and the following shall apply. 3.2 Portland Slag Cement An intimately interground mixture of Portland cement clinker and granulated slag with addition of gypsum and permitted additives or an intimate and uniform blend of Portland cement and finely ground granulated slag. 33. Portland Clinker Clinker, consisting mostly of calcium silicates, obtained by heating to incipient fusion a predetermined and homogeneous mixture of materials principally containing lime ( CaO ) and silica ( SiO, ) with a smaller proportion of alumina ( AlgO ) and iron oxide ( FezOI ). 3.4 Granulated Slag Slag in granulated form is used for the manuf?cture of hydraulic cement. Slag is a non-metallic product consisting essentially of glass containing silicates and alumino-silicates of lime and other bases, as in the case of blastfurnace slag, which is developed simultaneously with iron in blastfurnace or electric pig iron furnace. Granulated slag is obtained by further processing the molten slag by rapidly chilling or quenching it with water or steam and air. 4 MANUFACTURE 4.1 Portland slag cement shall be manufactured either by intimately intergrinding a mixture of Portland cement clinker and granulated slag with addition of gypsum ( natural or chemical ) or calcium sulphate, or by an intimate and uniform blending of Portland cement and finely ground A granulated slag, so that the resultant mixture would produce a cement capable of complying with this specification. No material shall be added other than gypsum ( natural or chemical ) or water or both. However, when gypsum is added it shall be in such amounts that the sulphur trioxide ( SO? ) in the cement produced does not exceed the ltmits specified in 5.2. Besides,not more than one percent of air-entraining agents or surfactants which have proved not to beharmful. may be added. The slag constituent shall be not less than 25 percent nor more than 65 percent of the PortJand slag cement. 5 CHEMICAL REQUIREMENTS
5.1 Portland cement clinker used in the manufacture of Portland slag cement shall comply in all respects with the chemical requirements specified for the 33 grade ordinary Portland cement in IS 269 : 1989, and the purchaser shall have the right, if he so desires, to obtain samples of the clinker used in the manufacture of Portland slag cement. 5.2 The Portland slag cement shall comply with the following chemical requirements when tested in accordance with the methods given ip IS 4032 : 1985: Percent, Max Magnesium oxide ( MgO ) Sulphur trioxide ( SO, ) Sulphide sulphur ( S ) Loss on ignition Insoluble residueNOTES 1 Total chloride content in cement rball not exceed 0.05 percent by mass for cement used in prestressed concrete structures and long rpan reinforced concrete structures. ( Method of test for determination of chloride content in cement is given in IS 12423 : 1988. ) 2 The limit of total chloride content in cement for use in plain and other reinforced concrete structures is being reviewed. Till that time, the limit may be mutually agreed to between the purchaser and the manufacturer. 3 Granulated slag conforming to IS I2i)89 : 1987 bar been found suitable for the manufacture of Portland slag cement.
80 3-o 15 50 4d
IS 455 : I989 6 PHYSICAL REQUIREMENTS 6.1 FinenessNOTES
When tested for fineness in terms of specific surface by Blaines Air permeability method described in IS 4031 ( Part 2 ) : 1988, the specific surface of slslg cement shall be not less than 225 m/kg.6.2 Soundness
Standard sand shall conform to IS 650 : 1966. of water required to produce a patteof standard consistency (see 11.3).2 P ijFthe percentage
6.2.1 When tested by Le-Chatelier method and autoclave test described in IS 4031 ( Part 3 ) : 1988, unaerated Portland slag cement shall not have an expansion of more than 10 mm and 08 Percent respectively. 184.108.40.206 In the event of cements failing to comply with any one or both the requirements specified in 63.1, further tests in respect of each fail&e shall be made as described in IS 4031 ( Part 3 ) : 1988 from another portion of the same sample after aeration. The aeration shall be done by spreading out the sample to a depth of 75 mm at a relative humidity of 50 to 80 percent fo,r a total period of 7 days. The expansion of cements so aerated shall be not more than 5 mm and 06 percent when tested by Le-Chatelier method and autoclave test respectively. 6.3 Setting Time The setting time of slag cement, when tested by the Vicat apparatus method described in 1S 4031 ( Part 5 ) : 1988, shall be as follows: Not less than a) Initial setting time 30 minutes Not more than b) Final setting time 600 minutes 6.3.1 If cement exhibits false set, the ratio o